Received: October 6, 2008 Accepted: December 8, · PDF fileRMZ – Materials and...
Embed Size (px)
Transcript of Received: October 6, 2008 Accepted: December 8, · PDF fileRMZ – Materials and...
420RMZ Materials and Geoenvironment, Vol. 55, No. 4, pp. 420431, 2008
Original scientific paper
Processing of PK 324 Duplex Stainless Steel: Influence of aging temperature and cooling rates on
precipitation - preliminary results
Preoblikovanje dupleksnega nerjavnega jekla PK 324: Vpliv temperature staranja in ohlajevalnih hitrosti na
izloanje preliminarni rezultati
MaTeV Fazarinc1, TaTjana VeKo PirToVeK1, DaViD BoMBa1, Goran KuGler1, Milan Terelj1
1University of Ljubljana, Faculty of Natural Sciences and Engineering, Department of Material Science and Metallurgy, Akereva cesta 12, SI-1000 Ljubljana, Slovenia;
E-mail: firstname.lastname@example.org, email@example.com, firstname.lastname@example.org, email@example.com, firstname.lastname@example.org
Received: October 6, 2008 Accepted: December 8, 2008
Abstract: Knowledge on precipitation phenomena in the PK 324 duplex stainless steel (DSS) is an important step in improving its final microstructure in the production process. Due to increased content of Cr, Ni and C the DSS exhibits complex microstructure, consisting of ferrite, austenite, intermetallic phases (sigma) and carbides. Several tests were applied in order to obtain necessary knowledge for improving the processing of the DSS. Aging-treatment tests re-vealed that sigma phase precipitated in the range between 680 C and 900 C. Additionally, the influence of cooling rates on the precipitation and transforma-tion behaviour of samples, previously aged in the range between 950 C and 1300 C, has been studied. With sufficiently high cooling rates the precipitation of sigma phase could be reduced to negligible values.
Izvleek: Razumevanje izloanja v dupleksnih nerjavnih jeklih PK 324 je pomemben korak k izboljavi konne mikrostrukture v procesu izdelave. Zaradi poviane koncentracije Cr, Ni in C tvori ta vrsta jekel kompleksno mikrostrukturo, ki je sestavljena iz ferita, avstenita, intermetalnih spojin (-faza) in karbidov. Iz-vedenih je bilo ve razlinih preizkusov, ki so sluili za nabiranje potrebnega znanja za izboljanje procesov izdelovanja teh jekel. S staranjem je bilo ugo-tovljeno, da se -faza izloa v temperaturnem intervalu med 680 C in 900 C. Dodatno je bila narejena e analiza vpliva ohlajevalnih hitrosti na vzorce, ki so bili predhodno starani v temperaturnem intervalu med 950 C in 1300 C. Pokazalo se je, da se je mogoe izogniti izloanju -faze z zadostno visoko ohlajevalno hitrostjo.
421Processing of PK 324 Duplex Stainless Steel: Influence of aging...
RMZ-M&G 2008, 55
Key words: PK 324 duplex stainless steel, aging treatment, cooling rates, pre-cipitation
Kljune besede: dupleksno nerjavno jeklo PK 324, staranje, ohlajevalne hitrosti, precipitacija
C or 950 C, respectively. The precipitation takes place on grain boundaries between the ferrite and austenite grains as well as on other incoherent boundaries (non-metallic inclusions). The -phase is one of the most influential phases according to the Fe-Cr binary system. It usually precipitates in the temperature range between 600 C and 1000 C, is very brittle and consequently increases the hardness of stainless steel but decreases ductility, toughness, corrosion resistance and consequently cold and hot deformability. Cooling rate influences the amount of precipitated carbides as well as the amount of sigma and other phases and consequently the obtained mechanical properties. Thus an appropriate processing parameters should be chosen in order to obtain the desired properties of the stainless steel in question that are needed in further processing steps for its quality production. After hot forming, cold forming is usually applied during the manufacturing of items whit fine dimensions (8 mm wire). The cold formability of stainless steel is highly influenced by present sigma phase as well
Table 1. Chemical compositions of various batches, used in our experimentsTabela 1. Kemina sestava razlinih ar, uporabljenih pri preizkusih
1 13 0.12 0.39 29.66 1.87 10.00 0.17 0.003 0.028 0.024 0.15
2 90 0.10 0.22 30.1 1.96 9.66 0.32 0.02 0.032 0.006 0.19
3 cast 0.10 0.26 30.1 1.91 9.5 0.04 0.004 0.020 0.007 0.06
Duplex stainless steels, composed manly of austenite and ferrite grains, posses excellent corrosion resistance as well as mechanical properties, i.e. good ductility and strength, where austenite contributes to the ductility while ferrite, which is harder, improves the strength and the welding characteristics. In the temperature range between 500 C and 1100 C the precipitation of secondary phases such as sigma phase () - (FeNi)x (CrMo)y intermetallic compound, chromium nitride (Cr2N), secondary austenite (2) and Chi phases () takes place in this type of stainless steels. When the composition is changed in the nominal concentration region the range of precipitation usually changes. Larger content of the ferrite-stabilizing elements, such as Mo and Si promote the -phase precipitation during the cooling process, while on the other hand the austenite-stabilizing elements, such as Ni, Mn, C and N reduce the -phase precipitation. Type M7C3 and M23C6 carbides usually commence to precipitate at temperatures bellow 1100
422 Fazarinc, M., VeKo PirToVeK, T., BoMBa, D., KuGler, G., Terelj, M.
RMZ-M&G 2008, 55
as by present carbides [1-14]. PK 324 is a ferrous alloy, usually used as welding material, grouped among super duplex stainless steel (DSS). Its produc-tion is still characterised by appearance of cracks as a consequence of precipitation processes. Thus this paper presents the results of influence of aging temperatures and cooling rates on the transformation and precipitation processes.
Applied materials, methods of characteri-zation and analysesThe specimens made of PK 324 DSS and applied in testing were cut from a rolled wire with diameter = 13 mm (Batch no. 1), from a square rod (90 mm x 90 mm, Batch no. 2) and from 380 kg ingots pre-pared in a vacuum electric furnace (Batch
Figure 1. Observed macrostructures on the cross sections of the PK 324 DSS ingot; a) in the ingot head (G), and b) in the ingot foot (N)Slika 1. Optina makrostruktura prenega prereza ingota jekla PK 324; a) glava ingota (G) in b) noga ingota (N)
no. 3). Chemical compositions of the ap-plied batches of the PK 324 DSS are given in Table 1. They differed from the stand-ard DSS since they contained higher mass fraction of C (over 0.1 %), Cr (about 30 %), and Ni (about 10 %). An isopleths cross section of the Fe-Cr-Ni ternary dia-gram at 8 % Ni is given in . (OM) ZEISS JENA VERT apparatus was applied for the light microscopy. Muraka-mis etchant (KleMM ) was used to tint phase grey, phase brown, carbides red, green and blue, while phase remained uncoloured. Further, XRD was used to ver-ify the percentage of phases in the micro-structure. Chemical compositions of the , , phases and of carbides were deter-mined with the EDS. Microanalyses were performed using the Leitz - AMR 1600 T scanning electron microscope and using the PGT IV EDX system. Figure 1a and b present the macrostruc-
423Processing of PK 324 Duplex Stainless Steel: Influence of aging...
RMZ-M&G 2008, 55
tures in the cross-sections in the ingots head (in the text marked with G) and in the ingots foot (in the text marked with N), re-spectively. Figure 1a made evident that an area 5 mm below the surface of the ingot consists of globular grains. Towards the in-got centre, a 10 mm wide area consisting of dendritic grains can be observed while the areas further towards the centre con-tain equiaxial grains that gradually change into globular grains in the centre of ingots head. The macrostructure of the cross sec-tion of ingot foot is presented in Figure 1b. The 5 mm wide area of globular grains in the outer part of ingot was clearly visible. Towards the ingot centre this area is fol-lowed by a 30 mm wide area of dendritic grains that gradually change into equiaxial grains and finally globular grains are found in the centre of ingots foot.The calculated value for Crekv/Niekv ratio according to the equation given in  is 2.3, pointing to the presence of both phases at room temperature. During the solidification process ferrite dendrites form first. After the solidifica-tion is complete the alloy consisted only of ferrite grains. Further cooling causes the
transformation and afterwards, due to the decreased solubility of C in austenite, precipitation of carbides takes place. With further cooling the decomposition of fer-rite according to the + eutectoid reaction takes place. During the cooling process the precipitation of carbides and of phase also takes place. Final microstruc-ture consists of -phase in the interdendritic spaces, phases and inside the dendrite grains, intermetallic phases (phases and ) and eutectic carbides. Figure 2a shows the final as-cast microstructure of the batch no. 3 taken from the ingot centre. Type M7C3 and M23C6 carbides predominately precipitate on the / boundaries in the in-terdendritic spaces (due to the segregation of C during the solidification process) and in a smaller extent also inside the grains close to the / boundaries while -phase precipitates in the ferrite area. Measured volume fraction of ferrite in the ingot cen-tre was about 48 %, austenite about 52 % and below 1 % of sigma phase and car-bides at room temperature. In the samples that were taken from the ingot surface the